Limestone Mold Jerusalem Stone LS 1302
Limestone Mold. Jerusalem Stone LS 1302
Mold size 2 SQ.FT(0.185m2). approximate.
Measurements - 24 3/4” X 13” X 1" (63cm X 33cm X 2.5cm)
Mold's sections — 1
Section dimensions: Approx. size 23 1/4” X 11 3/4” X 1/2 (59cm X 30 cm X 1 cm).
We offer the molds of the same stone style in several types. Each mold differs from each other by the texture of the stone. You may create a bigger variety of the stones for your product due to appliance of more than one mold.
LS 1302 Stone-casting Instructions:
Always apply release agent to your mold prior to casting concrete.
LS 1302 mold casting weight is about 7.88 lbs. (3.58 kg.)
We use this 1:2 cement to filler ratio mix : (you can also mix 1-part Portland cement to 3 parts sand [filler], but plasticizer and water has to be re-calculated by cement weight)
2.63 lbs (1.19 kg) Portland cement (white for light stone colors, gray for dark stone colors)
5.25 lbs (2.39 kg) Sand (20-30 mesh recommended. Silica sand or "all-purpose" sand works great)
10.51 oz (0.29 L) Water (We recommend water to be 20%-30% of cement weight.) (If your mix is too liquid, use less water.)
0.42 oz (11.93 g) Super-plasticizer (Superplasticizer's dosage rate is 0.5% -1% of cement weight. We are using 1%)
For best result always add dry pigments to your mix prior to adding the water. Mix concrete with pigment and additives for a few minutes, then add water (mix at least 3-5 minutes). You can also add Super plasticizer to the water 10-15 minutes prior to casting, then mix with dry ingredients.
Please note: Concrete minimum mixing time is 3 minutes (it takes a few minutes until Super Plasticizer absorbs into the cement and start reaction)
To color different molds sections, brush oxide pigment over the selected sections, then cast the concrete.
Cover the mold with plastic while it is curing. Remove the stone from the mold in 12-24 hours